This is an open access article published under a Creative Commons Attribution (CC-BY) License, which permits unrestricted use, distribution and reproduction in any medium, provided the author and source are cited.

Article pubs.acs.org/journal/apchd5

Gyroid Optical Metamaterials: Calculating the Eﬀective Permittivity of Multidomain Samples James A. Dolan,†,‡ Matthias Saba,§ Raphael Dehmel,‡,□ Ilja Gunkel,⊥ Yibei Gu,∥,# Ulrich Wiesner,∥ Ortwin Hess,§ Timothy D. Wilkinson,† Jeremy J. Baumberg,‡ Ullrich Steiner,⊥ and Bodo D. Wilts*,⊥ †

Department of Engineering, University of Cambridge, J.J. Thomson Avenue, Cambridge CB3 0FA, U.K. Nanophotonics Centre, Department of Physics, University of Cambridge, J.J. Thomson Avenue, Cambridge CB3 0HE, U.K. § Department of Physics, Imperial College, Prince Consort Road, London SW7 2BB, U.K. ⊥ Adolphe Merkle Institute, Chemin des Verdiers 4, 1700 Fribourg, Switzerland ∥ Department of Materials Science and Engineering, Cornell University, 330 Bard Hall, Ithaca, New York 14853-1501, United States ‡

S Supporting Information *

ABSTRACT: Gold gyroid optical metamaterials are known to possess a reduced plasma frequency and linear dichroism imparted by their intricate subwavelength single gyroid morphology. The anisotropic optical properties are, however, only evident when a large individual gyroid domain is investigated. Multidomain gyroid metamaterials, fabricated using a polyisoprene-b-polystyrene-b-poly(ethylene oxide) triblock terpolymer and consisting of multiple small gyroid domains with random orientation and handedness, instead exhibit isotropic optical properties. Comparing three eﬀective medium models, we here show that the specular reﬂectance spectra of such multidomain gyroid optical metamaterials can be accurately modeled over a broad range of incident angles by a Bruggeman eﬀective medium consisting of a random wire array. This model accurately reproduces previously published results tracking the variation in normal incidence reﬂectance spectra of gold gyroid optical metamaterials as a function of host refractive index and volume ﬁll fraction of gold. The eﬀective permittivity derived from this theory conﬁrms the change in sign of the real part of the permittivity in the visible spectral region (so, that gold gyroid metamaterials exhibit both dielectric and metallic behavior at optical wavelengths). That a Bruggeman eﬀective medium can accurately model the experimental reﬂectance spectra implies that small multidomain gold gyroid optical metamaterials behave both qualitatively and quantitatively as an amorphous composite of gold and air (i.e., nanoporous gold) and that coherent electromagnetic contributions arising from the subwavelength gyroid symmetry are not dominant. KEYWORDS: gyroid, optical metamaterial, eﬀective medium model, block copolymer, polymer self-assembly

E

permittivity and permeability in electromagnetic material design. Potential applications famously include cloaking devices and “superlenses”.2,3 However, of perhaps more immediate technological interest is the access to particularly large and small, or strongly anisotropic (e.g., hyperbolic), material parameters and their associated science and engineering.4 Whereas metamaterials that operate in the microwave regime have existed for decades, it is only relatively recently that

lectromagnetic metamaterials are artiﬁcially structured materials for which the electromagnetic response is a function of not only their chemical composition but also their structure.1 When the length scales of the constituent structural units are signiﬁcantly smaller than the wavelength of interest, the response of the metamaterial may be described by the homogenized eﬀective permittivity εeff(ω) and permeability μeff(ω). Metamaterials greatly expand the range of electromagnetic responses otherwise found in natural and synthetic bulk materials. They therefore oﬀer huge ﬂexibility to exploit exotic situations, or spatial arrangements of eﬀective © 2016 American Chemical Society

Received: June 14, 2016 Published: September 6, 2016 1888

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

Article

In this work, we investigate the optical properties of multidomain gold gyroid optical metamaterials fabricated from the alternating gyroid phase of a polyisoprene-bpolystyrene-b-poly(ethylene oxide) (ISO) triblock terpolymer. The specular reﬂection of the isotropic metamaterial is measured under a range of angles of incidence of light, and the resulting reﬂectance spectra are compared to those predicted by three of the simplest (and therefore most common) analytical eﬀective medium theories applicable to amorphous composites of spherical or ellipsoidal inclusions of one material in a host matrix of another. We show that a Bruggeman model with ellipsoidal inclusions is the only model considered that can reproduce the features present in the measured reﬂectance spectra of the investigated multidomain gold gyroid optical metamaterials and that such optical metamaterials behave substantially similarly to nanoporous gold.

advances in nanofabrication have allowed the manufacture of optical metamaterials.5 Due to the requirement that the structural units of a metamaterial be deeply subwavelength, ideally by an order of magnitude or more, optical metamaterials demand feature sizes on the length scale of tens of nanometers. However, many early top-down lithographic techniques either were intrinsically two-dimensional (e.g., a single material layer) or ventured into the third dimension only by tedious and nonscalable stacking of individual layers. These techniques are arguably still incapable of fabricating three-dimensional nanostructures over macroscopically large areas with suﬃcient speed and cost-eﬀectiveness to allow optical metamaterials to attain true technological relevance. Therefore, until recently, three-dimensional optical metamaterials presented a considerable challenge.6 Polymer self-assembly presents an alternative and particularly intriguing means by which to fabricate intricate one-, two-, and three-dimensional morphologies on the appropriate length scales, from which optical metamaterials may be replicated.7 Block copolymers are macromolecules consisting of two or more covalently linked homopolymers (“blocks”) that can microphase separate into various well-deﬁned morphologies due to the chemical dissimilarity between blocks. In block copolymers consisting of three distinct and sequential blocks (i.e., linear triblock terpolymers) one such morphology is the alternating gyroid: two single gyroid networks, each composed of one block, separated by a matrix of the third. The single gyroid is a continuous, chiral, and triply periodic cubic network with a constant mean curvature surface that is found in a range of natural and synthetic self-assembled systems.8 As the two single gyroid networks in the alternating gyroid are chemically distinct, it is possible to selectively remove just one such network and use the remaining voided terpolymer as a sacriﬁcial template for metal deposition.9,10 It was using this technique that Vignolini et al. fabricated the ﬁrst truly threedimensional self-assembled optical metamaterial: a gold single gyroid with a ∼50 nm unit cell size and 30% ﬁll fraction.11 Gyroid metamaterials possess a range of optical properties not exhibited by the pure metal, including an unambiguous optical anisotropy.8 Large individual domains exhibit a signiﬁcantly decreased plasma frequency and linear dichroism, evidenced by the shift of the extinction peak by up to 100 nm upon rotation under linearly polarized light.11 Both the plasma frequency and the linear dichroism are additionally a function of the unit cell size, ﬁll fraction, and dielectric environment.12,13 Although much is now known about the optical properties of gyroid metamaterials, suitable estimates of the eﬀective material parameters remain elusive, thereby hindering a true appraisal of the metamaterial’s potential utility. A trihelical metamaterial (THM) model of the gyroid as periodic disconnected helices allows the analytical derivation of the permittivity, permeability, and chiral coupling parameter.14,15 From these the plasma frequency of the metamaterial and its variation with unit cell size, ﬁll fraction, and dielectric environment can be successfully predicted.12 However, the THM model does not describe the linear dichroism of gyroid metamaterials, and the model is unsuitable to average over an ensemble of small domains of random orientation and handedness. It is therefore of great interest to correctly identify the eﬀective material parameters of gyroid metamaterials and to understand to what extent the ordered subwavelength structure continues to aﬀect the optical response when the macroscopic order is not long range.

■

EFFECTIVE MEDIUM THEORIES For a material that is homogeneous at a particular length scale, its physical properties may be described by a reduced set of eﬀective material parameters.16 Eﬀective medium theories are approximate analytical means to ascribe a homogeneous (although potentially anisotropic) material parameter, in this case εeff(ω), to a heterogeneous mixture of two or more components.1 Such theories are anticipated to hold when the inhomogeneity length scale of the material and the local variation in the electric ﬁeld are both signiﬁcantly smaller than the wavelength of interest.17 Although numerous approaches of varying complexity exist, the two considered in this work are arguably the most prevalent theories: the Maxwell−Garnett theory for spherical inclusions and the Bruggeman theory.1,17 Maxwell−Garnett Theory: Case of Spherical Inclusions. The simplest form of the Maxwell−Garnett eﬀective medium theory considers spherical inclusions of one material in a host matrix of another material (Figure 1a). The eﬀective permittivity is found by solving the following implicit equation:1 (ε1(ω) − ε2(ω))f1 ε2(ω) + (ε1(ω) − ε2(ω))A +

ε2(ω) − εeff (ω) =0 ε2(ω) + (εeff (ω) − ε2(ω))A

(1)

where εeff(ω) is the (isotropic) eﬀective permittivity of the composite, ε1(ω) is the permittivity of the ﬁrst component (the inclusion), ε2(ω) is the permittivity of the second component (the host), f1 is the volume fraction of the ﬁrst component, A is the depolarization factor (1/3 for spherical inclusions), and ω is frequency. The depolarization factor relates the dipole moment of a dielectric ellipsoid to the applied external electric ﬁeld and varies from 0 (disks) to 1 (wires). The above theory is strictly valid only when the volume ﬁll fraction of the inclusions is small. As a result, the above equation is not invariant under the transformation ε1 ↔ ε2 and f1 ↔ f 2. Asymmetric formulations such as this are only valid for low volume fractions of the polar phase (see, for example, Table 1 in ref 18). Nonetheless, the Maxwell−Garnett eﬀective medium theory should be considered due to its widespread usage and having previously been employed to justify the diﬀering behavior of gold gyroid metamaterials from an amorphous composite.11 1889

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

Article

composite, it is possible to extend the theory to take anisotropy of the inclusions into account. This is done by modeling such inclusions as aligned ellipsoids with semiaxes ak. In such a case the depolarization factor A in eq 2 is replaced by Ak =

a1a 2a3 2

∫0

∞

du (ak2

+ u)

(a12

+ u)(a 22 + u)(a32 + u)

where Ak is the depolarization factor for light linearly polarized along the kth axis of an aligned ellipsoidal inclusion. Note that the derived eﬀective permittivity is hence only valid for that same relative orientation of linearly polarized light and the eﬀective permittivity of the material is anisotropic (i.e., when all ellipsoidal inclusions are assumed to be aligned). However, it is also possible to deﬁne a macroscopically isotropic eﬀective permittivity while allowing for microscopic anisotropy if the ellipsoidal inclusions are assumed to be randomly oriented in the composite (Figure 1c). In such a case, the eﬀective permittivity is derived by solving the following implicit equation (see Supporting Information): 3

∑ k=1

=0

(3)

RESULTS An optical and electron micrograph of the multidomain gyroid metamaterial, the geometry of the experiment, and the resulting reﬂectance spectra for transverse magnetic (TM) and transverse electric (TE) polarizations of incident light are shown in Figure 2. The optical micrograph captured under linearly polarized light (Figure 2a) highlights the light orange color of the metamaterial, and the electron micrograph of an individual domain (Figure 2b) is consistent with the gyroid nanostructure previously observed for this terpolymer.11−13 The small size and multiplicity of the domains can be more clearly seen in Figure S1. Both TM (Figure 2d) and TE (Figure 2e) reﬂectance spectra are qualitatively similar to those of bulk gold (Figure S2), insofar as they exhibit low reﬂectance at shorter wavelengths and increased reﬂectance at longer wavelengths across all angles of incidence. (Note that in Figures 2−5, reﬂectance spectra are plotted on a log scale as they exhibit spectral features that span multiple orders of magnitude.) In bulk gold, these features are attributable to interband transitions and the plasma frequency, respectively. However, the measured spectra diﬀer quantitatively from those of bulk gold due to both a lowered eﬀective plasma frequency and their variation with angle of incidence. Otherwise, the spectra exhibit the general decrease (increase) in reﬂectance for

εeff (ω) + (ε1(ω) − εeff (ω))A =0

εeff (ω) + (ε2(ω) − εeff (ω))Ak

■

(ε1(ω) − εeff (ω))f1

εeff (ω) + (ε2(ω) − εeff (ω))A

(ε2(ω) − εeff (ω))f2

where εeff(ω), ε1(ω), ε2(ω), f1, f 2, and ω are as deﬁned above and Ak are the three depolarization factors corresponding to the geometry of the ellipsoidal inclusions (A1 + A2 + A3 = 1). Note that this equation is identical for both a polycrystalline sample consisting of numerous randomly oriented anisotropic domains and a composite sample consisting of equal amounts of three isotropic constituents of diﬀering permittivities or depolarization factors.16 Note also that the Maxwell−Garnett theory may similarly be extended to take into account microscopic anisotropy (vide inf ra).

Bruggeman Theory: Case of Spherical Inclusions. We adopt here a version of the Bruggeman eﬀective medium theory, in which all constituents of the composite are treated symmetrically. If the inclusions are again assumed to be spherical (Figure 1b), the eﬀective permittivity is found by solving the following implicit equation (see Supporting Information for more information):18

(ε2(ω) − εeff (ω))f2

εeff (ω) + (ε1(ω) − εeff (ω))Ak

+

Figure 1. Sketches of the mathematical representations of various eﬀective medium theories. (a) Maxwell−Garnett, eq 1, where the eﬀective permittivity (εeff) is derived by considering spherical inclusions (A = 1/3) of one material (ε1) in a host matrix of another (ε2). (b) Bruggeman (A = 1/3), eq 2, where the eﬀective permittivity (εeff) is derived by averaging over single inclusions (ε1 and ε2) individually embedded in an eﬀective medium consisting of all other inclusions (εeff). (c) Bruggeman (Ak), eq 3, where the eﬀective permittivity (εeff) is derived analogously to the case where A = 1/3 except that all individual spherical inclusions are replaced by randomly oriented ellipsoids. (d) The single gyroid morphology for which an eﬀective medium theory is sought.

+

(ε1(ω) − εeff (ω))f1

(2)

where εeff(ω), ε1(ω), ε2(ω), f1, A, and ω are deﬁned as above, and f 2 = 1 − f1 is the volume ﬁll fraction of the second component. Note that the above equation is now invariant under the transformation ε1 ↔ ε2 and f1 ↔ f 2, indicating that the Bruggeman eﬀective medium theory is applicable for any given volume ﬁll fraction. It is therefore anticipated that this simplest form of the Bruggeman theory may more accurately model the behavior of 30% ﬁll fraction gyroid metamaterials, such as those considered here. Bruggeman Theory: Case of Ellipsoidal Inclusions. Although the Bruggeman eﬀective medium theory is insensitive to the absolute size of the subwavelength inclusions of a 1890

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

Article

Figure 2. Gyroid optical metamaterials: optical and electron micrographs, experiment geometry, and measured reﬂectance spectra. (a) Optical micrograph of multidomain gold gyroid metamaterial under linearly polarized light (scale bar 100 μm). (b) Electron micrograph of an individual domain of the sample (scale bar 200 nm). (c) Specular reﬂectance spectra of the gyroid metamaterial are measured as a function of angle of incidence between 15° and 65° and 450 and 800 nm. Although a single gyroid domain is shown for clarity, the measurement spot size in fact encompasses a large number of randomly oriented gyroid domains. (d) Reﬂectance spectra as a function of angle of incidence for transverse magnetic (TM) polarized light (log color scale extends from −1.8 to −0.1). (e) The same for transverse electric (TE) polarized light (log color scale extends from −1.8 to −0.1).

Figure 3. Comparison of measured and modeled TM reﬂectance spectra as a function of angle of incidence using three eﬀective medium theories. (a) Measured reﬂectance spectra for transverse magnetic (TM) polarized light repeated from Figure 2d (log color scale extends from −1.8 to 0). (b) Reﬂectance spectra generated using the Maxwell−Garnett theory (log color scale extends from −6.0 to −1.0). (c) The same generated using the Bruggeman theory and A = 1/3, i.e., spherical inclusions (log color scale extends from −2.0 to −0.8). (d) The same generated using the Bruggeman theory and A1 = 0.66, A2 = 0.34, and A3 = 0, i.e., ellipsoidal inclusions (log color scales extends from −1.9 to −0.6).

TM (TE) polarized light with increasing angle of incidence, with an eﬀective Brewster’s angle of ∼50°. A comparison between the measured and modeled reﬂectance spectra across all wavelengths and angles of incidence for TM polarized light is shown in Figure 3; the same for TE polarized light is shown in Figure S3. The eﬀective permittivity εeff(ω) used to generate the modeled spectra in Figure 3b was calculated using the Maxwell−Garnett theory by setting ε1(ω) = εAu(ω), ε2(ω) = 1, f1 = 0.3, and A = 1/3 (i.e.,

spherical inclusions) in eq 1. Clearly the Maxwell−Garnett eﬀective medium theory is a poor model for the eﬀective permittivity of the gyroid metamaterial, as it predicts a striking dip in reﬂectance at an eﬀective Brewster’s angle of ∼60°, which is entirely absent in the measured data. Despite also assuming spherical inclusions, the eﬀective permittivity calculated using the Bruggeman theory, by again setting ε1(ω), ε2(ω), f1, and A as above in eq 2, results in a far better qualitative match between the measured and modeled 1891

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

Article

Figure 4. Variation in normal incidence reﬂectance spectra and plasma edge as a function of host refractive index. (a) Measured reﬂectance spectra at normal incidence for 30% ﬁll fraction gold gyroid metamaterials inﬁltrated with media of refractive indices 1.0 (solid line), 1.33 (dashed line), 1.5 (dotted-dashed line), and 1.7 (dotted line) and the associated plasma edge of each spectrum in nanometers (labeled vertical lines of the same style). Data are reproduced from Salvatore et al.12 (b) Modeled normal incidence reﬂectance spectra using the optimized Bruggeman model where ε2(ω) of eq 3 is set to 1.02 (solid line), 1.332 (dashed line), 1.52 (dotted-dashed line), and 1.72 (dotted line) and the associated plasma edge of each spectrum in nanometers (labeled vertical lines of the same style). (c) Plasma edge against refractive index of host for measured (Expt.) and modeled (Brugg.) spectra and the relationship predicted by the trihelical metamaterial (THM) model, reproduced from Salvatore et al.12

Figure 5. Variation in normal incidence reﬂectance spectra and plasma edge as a function of gold volume ﬁll fraction. (a) Measured normal incidence reﬂectance spectra of gold gyroid metamaterials with volume ﬁll fractions of 30% (solid line), 45% (dashed line), 60% (dotteddashed line), 75% (dotted line), and 90% (solid line with circles) and the associated plasma edge of each spectrum in nanometres (labeled vertical lines of the same style). Data reproduced from Salvatore et al.12 (b) Modeled normal incidence reﬂectance spectra using the optimized Bruggeman model where f1 of eq 3 is set to 0.30 (solid line), 0.45 (dashed line), 0.60 (dotted-dashed line), 0.75 (dotted line), and 0.90 (solid line with circles) and the associated plasma edge of each spectrum in nanometers (labeled vertical lines of the same style). (c) Plasma edge against volume ﬁll fraction of gold for measured (Expt.) and modeled (Brugg.) spectra and the relationship predicted by the trihelical metamaterial (THM) model, reproduced from Salvatore et al.12

reﬂectance spectra (Figure 3c). The global reﬂectance minimum at ∼50° between 450 and 500 nm is reproduced well. However, the spectra still exhibit a decrease in reﬂectance at long wavelengths and high angles of incidence, which is not present in the experimental data. This decrease in reﬂectance is absent in the reﬂectance spectra of Figure 3d, which uses our microscopically anisotropic Bruggeman theory. These spectra were modeled by setting ε1(ω), ε2(ω), and f1 as above and A1 = 0.66, A2 = 0.34, and A3 = 0 in eq 3. These depolarization factors were found by performing a constrained optimization to ﬁt the TM reﬂectance spectra generated by the model to the measured data (see Experimental Methods). A quantitative comparison of the goodness of ﬁt of each model is presented in Table 1. Cost functions f(A) (see Experimental Methods) are tabulated not only for TM but also for TE polarization using the depolarization factors derived from the TM measurements. Note that the cost function evaluated for TE polarization using the depolarization factors derived from the TM measurements (A1 = 0.66, A2 = 0.34, and A3 = 0) is only 0.66% larger than the same cost function evaluated for TE polarization using the depolarization factors derived from the TE measurements (A1 = 0.70, A2 = 0.30, and

Table 1. Table of Cost Functions f(A) (See Experimental Methods) Associated with the Various Eﬀective Medium Theories (model), Equations (eq), Polarizations (pol), and Vector of Depolarization Factors (A)a

a

model (eq)

pol

A

f(A)

Max.−Garn. (1) Brugg. (2) Brugg (3) Max−Garn (1) Brugg (2) Brugg (3)

TM

1/3 1/3 [0.66, 0.34, 0] 1/3 1/3 [0.66, 0.34, 0]

2.02 0.28 0.12 0.34 0.08 0.04

TE

A lower value of cost function indicates a better ﬁt.

A3 = 0). This would not in general be the case (e.g., for an anisotropic sample). Both ﬁts yield A3 = 0, which thus selects a wire (i.e., a uniaxially inﬁnitely extended ellipsoid) with an elliptical cross-section. It is therefore clear that the microscopically anisotropic Bruggeman model consisting of randomly oriented wire inclusions is the best of the three eﬀective medium models considered and that only a single set of 1892

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

■

depolarization factors, A1 = 0.66, A2 = 0.34, and A3 = 0, is appropriate to model both TM and TE measurements. A good model for the eﬀective permittivity of the gyroid metamaterial should be capable of reproducing not only the measured reﬂectance spectra presented in this work but also the previously reported behaviors as a function of refractive index of the host and volume ﬁll fraction of gold. Figure 4 compares measurements performed by Salvatore et al. on 30% ﬁll fraction gold gyroids inﬁltrated with various refractive index media with the optimized Bruggeman model.12 Following the convention in that work, each normal incidence spectrum is characterized by its plasma edge, the wavelength of the point of inﬂection of the reﬂectance spectrum. In the simplest Drude model of the permittivity of metals, the plasma wavelength is the wavelength at which the permittivity changes from positive to negative and is characteristic of the density and eﬀective mass of the free electrons in the particular metal. The plasma edge is not the plasma wavelength but behaves similarly and may be more readily and systematically identiﬁed from experimental data than the plasma wavelength (see for example Figure S6 of ref 12). Figure 4a reproduces the reﬂectance spectra measured by Salvatore et al. upon inﬁltration of the gyroid metamaterial with media of refractive indices nfill = 1.0, 1.33, 1.5, and 1.7 and indicates the plasma edge in each case (the labeled vertical lines). Note how the plasma edge is red-shifted with increasing host refractive index. Figure 4b plots equivalent normal incidence reﬂectance spectra derived using the optimized Bruggeman model with ε2(ω) of eq 3 set to n2fill, respectively. Again the plasma edge is red-shifted with increasing host permittivity. Although the measured and modeled plasma edges do not perfectly coincide, it is clear from Figure 4c that the modeled plasma edges are within experimental error for each refractive index. Therefore, despite the dissimilarity between the measured and modeled normal incidence reﬂectance spectra, the model successfully predicts the plasma edge of the gold gyroid metamaterial. Furthermore, the optimized Bruggeman model performs better in this respect than the trihelical metamaterial analytical model, also reproduced from Salvatore et al. and shown in Figure 4c.12 The results of the optimized Bruggeman model may also be compared to previously measured data where the volume ﬁll fraction of gold is varied. Figure 5a shows normal incidence reﬂectance spectra from Salvatore et al. as the volume ﬁll fraction of the gold gyroid is increased from 30% to 90%. Only four of the ﬁve plasma edges are shown, since those for the 75% and 90% ﬁll fraction gyroids are within 2 nm of one another. Whereas the plasma edge is red-shifted with increasing refractive index of the host, it is blue-shifted as the ﬁll fraction increases and the reﬂectance of the gyroid metamaterial tends toward that of bulk gold. Figure 5b plots equivalent normal incidence reﬂectance spectra calculated from the optimized Bruggeman model. Here only two of the ﬁve plasma edges are shown, as all of those corresponding to ﬁll fractions above 30% are extremely close (within 2 nm). Again the plasma edge is blue-shifted with increased ﬁll fraction, as it was in the measured spectra. However, as can be seen in Figure 5c, there is signiﬁcant deviation between the measured and predicted plasma edges for intermediate ﬁll fractions between about 40% and 70%. Outside of this region (i.e., at low and high ﬁll fractions) the optimized Bruggeman model performs well and is comparable with the THM model.

Article

DISCUSSION

The failure of the Maxwell−Garnett theory to describe multidomain gyroid samples is perhaps not surprising, since its validity is limited to a low volume fraction of spherical dielectric inclusions that are spatially separated. The gyroid samples considered here consist however of an interconnected, percolating network of gold struts. The better description of the experimental system by the Bruggeman model with spherical inclusions arises primarily from the fact that this model retains it validity for a high density of scatterers, expressed in the model by the ﬁll fraction. The results of Figure 3 indicate that a model based on an eﬀective medium approach is able to approximate the random multidomain gyroid network, despite the morphological dissimilarity. While a model with a larger number of free parameters (i.e., the three depolarization factors) is expected to improve the level of agreement with the data, it is revealing that ﬁts of both reﬂected TE and TM polarized light result always in zero values for one of the depolarization factors Ak. Since Ak < 1/3 corresponds to a prolate ellipse, with a divergence for Ak → 0, the optimization of the Bruggeman model with free Ak values results in an eﬀective medium consisting of randomly oriented wires of elliptical cross-section (see Figure 6 inset). While a random wire assembly is a better description than isolated individual scatterers for an interconnected gyroid network, the good agreement between ﬁt and data is nevertheless surprising given that the Bruggeman theory does not model well percolating networks.19 Although allowing for microscopic anisotropy within the Maxwell−Garnett model (i.e., ellipsoidal inclusions) might similarly improve upon the results of the equivalent model with spherical inclusions, this variant of the Maxwell−Garnett model would still suﬀer from a limited validity because of the high volume ﬁll fractions of our samples and was therefore not considered. Like the classical wire-grid metamaterial, the gold gyroid metamaterial is shown to exhibit a strongly red-shifted plasma edge.20 The eﬀective permittivity εeff(ω) derived from the Bruggeman theory with optimized depolarization factors, shown in Figure 6a, has a crossover of the real part of the permittivity just below 650 nm (arrow). In contrast, the real part of the permittivity of the constituent gold does not cross the zero axis at any wavelength in the visible (inset). Notwithstanding the eﬀect of losses associated with the imaginary part of the permittivity, the gold gyroid metamaterial therefore behaves as both a dielectric (λ ≲ 650 nm) and metal (λ ≳ 650 nm) in the visible. In the simple Drude model of the permittivity of a metal, this crossover is associated with the plasma frequency (plasma wavelength), an association that is hard to isolate in more complicated models (e.g., Drude− Lorentz) or experimentally measured permittivities. The previously introduced plasma edge is thus useful to characterize the optical response of the gyroid metamaterial, despite the lack of a direct correlation with prominent features in the permittivity plots. The variation of the predicted real part of the permittivity with refractive index of the host and ﬁll fraction of gold is shown in Figure 6b and c, respectively. Although quantitatively distinct, it is clear that the general behaviors of both the plasma edge (Figures 4c and 5c) and the crossover wavelength (Figure 6b and c) are broadly similar. On the basis of this and the good ﬁt of the Bruggeman model to the specular reﬂectance spectra, we conclude that gyroid metamaterials 1893

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

Article

and the volume ﬁll fraction of gold near the top surface, accounting for the diﬀerences in the reﬂectivity. The relative decrease in the long-wavelength reﬂectance at high angles of incidence predicted by the Bruggeman model, more prominent when spherical inclusions are assumed and not present in the data, may similarly be a result of the gyroid metamaterial having a somewhat larger volume ﬁll fraction of gold at its surface compared with that expected from a planar cut across the gyroid morphology. Incorrect ﬁll fractions during optimization of the depolarization factors may also help to explain the relative inaccuracy of the model at intermediate ﬁll fractions (i.e., between about 40% and 70%) compared to the relative accuracy of the same model with respect to increasing refractive index of the host. However, to note that the fabrication of gyroid metamaterials with increased ﬁll fraction and the accurate measurement of the ﬁll fraction are diﬃcult compared to inﬁltration of the metamaterial with varying refractive index media.12 Results of the former experiments should therefore be treated with some caution. Finally, whereas all of the eﬀective medium models considered are insensitive to the absolute size of the subwavelength inclusions, it is known that the optical properties of gold gyroid metamaterials vary with unit cell size.12 The results presented here are therefore limited to gold gyroids with a similar unit cell size (i.e., ∼60 nm), although the methodology can of course easily be extended to gold gyroids of other unit cell sizes. Despite the potential shortcomings of the relatively simple analytical models employed here, the application of more complicated analytical models would not alter the current conclusion: that multidomain gold gyroid optical metamaterials behave substantially as if they were nanoporous gold.

■

Figure 6. Eﬀective permittivity of small domain gyroid metamaterials derived from the Bruggeman eﬀective medium theory. (a) Real (solid line) and imaginary (dashed line) parts of the eﬀective permittivity εeff(ω) calculated using the Bruggeman theory by setting ε1(ω) = εAu(ω), ε2(ω) = 1, f1 = 0.3, A1 = 0.66, A2 = 0.34, and A3 = 0 in eq 3. The insets are a sketch of the equivalent structure corresponding to the optimized Bruggeman model and the real (solid line) and imaginary (dashed lines) part of the permittivity of bulk gold εAu(ω). (b) Variation of the real part of the eﬀective permittivity with refractive index of the host medium. (c) Variation of the same with volume ﬁll fraction of gold.

CONCLUSION

In this work, the eﬀective permittivity of multidomain gold gyroid metamaterials was estimated by comparing the results of three eﬀective medium theories to measured specular reﬂectance spectra over a range of angles of incidence. We show that a microscopically anisotropic Bruggeman theory with wire inclusions provides the best ﬁt to the data and that the optimized depolarization factors imply a composite of randomly oriented gold wires of elliptical cross-section. That the averaged optical properties of multidomain gyroid metamaterials are well described by an eﬀective medium theory, including their variation with refractive index of the host and volume ﬁll fraction of gold, contradicts previous assertions that the subwavelength structure necessarily alone distinguishes gold gyroid metamaterials from amorphous nanoporous gold.11 This result is surprising, given the experimental results obtained for large individual gyroid domains.11 In particular, the gyrotropic transmission along one of the chiral gyroid axes that was attributed to the self-inductance of plasmon-polariton modes is not captured by the eﬀective medium model. If symmetry-related eﬀects of the intricate gyroid structure do indeed contribute to the optical properties of a macroscopic sample consisting of numerous randomly oriented domains, it seems that this contribution is averaged out through the random alignment of the multidomain gyroid assembly, as also appears to be the case for gyroid photonic crystals.29,30

averaged over many randomly oriented domains behave similarly to amorphous composites of air and gold (i.e., dilute metals) and therefore possess a similar response to nanoporous gold fabricated, for example, by dealloying.21−28 Although the optimized Bruggeman model is successful in predicting the optical properties of multidomain gold gyroid optical metamaterials (allowing to conclude that their optical properties are similar to nanoporous gold), it is by no means perfect, and various dissimilarities exist between the measured and predicted spectra. Surprisingly, the measured reﬂectance spectra are generally higher than those predicted. This is most likely caused by the details of the gyroid surface. For example, surface reconstruction (i.e., local reorientation) of the terblock terpolymer during thermal annealing can alter the in-coupling of light into the gyroid network. Alternatively, the details of the gyroid fabrication process might aﬀect the surface roughness 1894

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

■

Article

A1 + A 2 + A3 = 1

EXPERIMENTAL METHODS Fabrication. Gold gyroid metamaterial fabrication has been detailed elsewhere.11−13,31 In brief, samples are prepared using substrates of ﬂuorine-doped tin oxide (FTO)-coated glass (Solaronix) that have been cleaned using a piranha etch and immersed for 15 s in a 0.2% solution (v/v) of octyltrichlorosilane (Sigma-Aldrich) in anhydrous cyclohexane (SigmaAldrich). An 80 kg/mol polyisoprene-b-polystyrene-b-poly(ethylene oxide) triblock terpolymer with block volume fractions of 30%, 53%, and 17%, respectively (synthesized by anionic polymerization as detailed elsewhere32,33), is spun from a 10% (w/w) anhydrous anisole (Sigma-Aldrich) solution at 1200 rpm, resulting in an approximately 1 μm thick ISO ﬁlm as measured by thin ﬁlm interferometry. Samples are subsequently thermally annealed under vacuum at 180 °C for 30 min (ramp rate 150 °C/h), then allowed to cool over approximately 12 h. The polyisoprene block is degraded by exposure to UV light (VWR International, 254 nm, ∼50 mW/cm2) for up to 2 h and removed by dissolution in ethanol. The resulting template is ﬁlled by electrodeposition of gold (Metalor ECF60 and 0.5% (v/v) E3 brightener) at a constant potential of −0.8 V following a nucleation step (a cyclic voltammetry scan at a rate of 0.05 V/s with vertex potentials of 0, −1.2, and 0 V). The three-electrode cell consisted of the FTO-coated glass substrate as the working electrode, an evaporated gold thin ﬁlm as the counter electrode, and a saturated calomel reference electrode. Gold is grown both within and atop the polymer template, and the layer of excess bulk gold is cleaved at the interface between the nanostructured and bulk gold using Kapton tape, to ensure a smooth top surface (i.e., low surface roughness). Following electrodeposition, the remaining polymer template was removed by exposure to oxygen plasma for approximately 10 min (Diener MRC 100 at 100% power). The resulting gold single gyroid has a unit cell size of ∼60 nm and a ﬁll fraction of 30%.11,12 Characterization. Optical characterization is performed using an automated reﬂection goniometer with a ﬁxed illumination arm (QP600-2-SR-BX 600 μm core ﬁber and HPX-2000 Ocean Optics xenon light source). The sample and detection arm are arranged in the θ−2θ conﬁguration such that whenever the sample is tilted by an angle θ, the detection arm is tilted by an angle 2θ. The spectra are recorded by coupling the reﬂected light into an optical ﬁber (QP230-2-XSR 230 μm core) connected to a spectrometer (Ocean Optics QE6500) and are normalized at all angles of incidence with respect to the reﬂectance of a silver mirror. Linear polarizers are placed at the output of the illumination ﬁber and at the input of the detection ﬁber, ﬁxed to the illumination and detection arms, respectively. Spectra are recorded at angles of incidence between 15° and 65° in steps of 1°. The procedure is repeated for both TE and TM polarizations in parallel conﬁgurations (i.e., aligned polarizer and analyzer). Model. Where an eﬀective medium model requires ﬁtting, the MATLAB optimization toolbox is used to minimize the cost function: f (A) =

1 N×M

where A = [A1, A2, A3], Ak is the kth depolarization factor, λi is the ith wavelength, θinj is the jth angle of incidence, N is the total number of wavelengths, M is the total number of angles of incidence, and Rexp(λi, θinj ) and Rmodel(λi, θinj , A) are the experimental and modeled reﬂectance spectra, respectively. The modeled reﬂectance spectra are in turn calculated from the Fresnel equations for reﬂection from a semi-inﬁnite nonmagnetic homogeneous medium for TE: TE R model (λ i ,

θjin ,

A) =

nair cos(θjin) − neff (λi , A) cos(θjtr)

2

nair cos(θjin) + neff (λi , A) cos(θjtr)

and TM: TM R model (λ i ,

θjin ,

A) =

neff (λi , A) cos(θjin) − nair cos(θjtr)

2

neff (λi , A) cos(θjin) + nair cos(θjtr)

polarized light, where nair and neff(λi, A) are the refractive indices of air and the eﬀective medium respectively, and θtrj is the jth (complex) transmitted angle calculated by Snell’s law, i.e., nair sin(θjin) = neff (λi , A) sin(θjtr)

The assumption that the gold gyroid metamaterial appears semi-inﬁnite (and that the derived eﬀective permittivity is insensitive to ﬁlm thickness) is based upon the thickness of the ﬁlm (∼1 μm), the unit cell size (∼60 nm), and previous studies of ﬁlm thickness eﬀects in gold gyroid optical metamaterials,34 which indicate that the reﬂectance spectra do not change beyond a threshold sample thickness. The eﬀective medium models from which neff(λi, A) is derived require as an input the permittivity of bulk gold, εAu(ω), which is here taken as that measured by Olmon et al.35 Optimized depolarization factors are calculated for each polarization state of light.

■

ASSOCIATED CONTENT

S Supporting Information *

The Supporting Information is available free of charge on the ACS Publications website at DOI: 10.1021/acsphotonics.6b00400. Additional data related to this publication is available at the University of Cambridge data repository (http://dx.doi.org/10.17863/CAM.4376). Supplementary Figures S1−S3 and details on the derivation of the Bruggeman eﬀective medium theory (PDF)

■

AUTHOR INFORMATION

Corresponding Author

*E-mail: [email protected] Phone: +41 (0)26 300 89 69.

N

Present Addresses

∑×

□

Papierfabrik Louisenthal GmbH, 83701 Gmund a.T., Germany. # The Dow Chemical Company, 2301 N. Brazosport Boulevard, Freeport, Texas 77541, United States.

i=1

M

∑ (log10R exp(λi , θjin) − log10R model(λi , θjin , A))2 j=1

Notes

The authors declare no competing ﬁnancial interest.

such that 1895

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

■

Article

(19) Kirkpatrick, S. Percolation and conduction. Rev. Mod. Phys. 1973, 45, 574. (20) Pendry, J. B.; Holden, A. J.; Stewart, W. J.; Youngs, I. Extremely low frequency plasmons in metallic mesostructures. Phys. Rev. Lett. 1996, 76, 4773−4776. (21) Yu, F.; Ahl, S.; Caminade, A.-M.; Majoral, J.-P.; Knoll, W.; Erlebacher, J. Simultaneous excitation of propagating and localized surface plasmon resonance in nanoporous gold membranes. Anal. Chem. 2006, 78, 7346−50. (22) Dixon, M. C.; Daniel, T. A.; Hieda, M.; Smilgies, D. M.; Chan, M. H. W.; Allara, D. L. Preparation, structure, and optical properties of nanoporous gold thin films. Langmuir 2007, 23, 2414−22. (23) Maaroof, A. I.; Gentle, A.; Smith, G. B.; Cortie, M. B. Bulk and surface plasmons in highly nanoporous gold films. J. Phys. D: Appl. Phys. 2007, 40, 5675−5682. (24) Biener, J.; Nyce, G. W.; Hodge, A. M.; Biener, M. M.; Hamza, A. V.; Maier, S. A. Nanoporous Plasmonic Metamaterials. Adv. Mater. 2008, 20, 1211−1217. (25) Sardana, N.; Birr, T.; Schlenker, S.; Reinhardt, C.; Schilling, J. Surface plasmons on ordered and bi-continuous spongy nanoporous gold. New J. Phys. 2014, 16.06305310.1088/1367-2630/16/6/063053 (26) Sardana, N.; Heyroth, F.; Schilling, J. Propagating surface plasmons on nanoporous gold. J. Opt. Soc. Am. B 2012, 29, 1778. (27) Lang, X.; Qian, L.; Guan, P.; Zi, J.; Chen, M. Localized surface plasmon resonance of nanoporous gold. Appl. Phys. Lett. 2011, 98, 2009−2012. (28) Maaroof, A. I.; Cortie, M. B.; Smith, G. B. Optical properties of mesoporous gold films. J. Opt. A: Pure Appl. Opt. 2005, 7, 1464−4258. (29) Michielsen, K.; De Raedt, H.; Stavenga, D. G. Reflectivity of the gyroid biophotonic crystals in the ventral wing scales of the Green Hairstreak butterfly, Callophrys rubi. J. R. Soc., Interface 2010, 7, 765− 771. (30) Saba, M.; Wilts, B. D.; Hielscher, J.; Schröder-Turk, G. E. Absence of Circular Polarisation in Reflections of Butterfly Wing Scales with Chiral Gyroid Structure. Mater. Today: Proc. 2014, 1, 193− 208. (31) Farah, P.; Demetriadou, A.; Salvatore, S.; Vignolini, S.; Stefik, M.; Wiesner, U.; Hess, O.; Steiner, U.; Valev, V. K.; Baumberg, J. J. Ultrafast Nonlinear Response of Gold Gyroid Three-Dimensional Metamaterials. Phys. Rev. Appl. 2014, 2, 044002. (32) Bailey, T. S.; Pham, H. D.; Bates, F. A. Morphological Behavior Bridging the Symmetric AB and ABC States in the Poly(styrene-bisoprene-b-ethylene oxide) Triblock Copolymer System. Macromolecules 2001, 34, 6994−7008. (33) Bailey, T. S.; Hardy, C. M.; Epps, T. H.; Bates, F. S. A Noncubic Triply Periodic Network Morphology in Poly(isoprene-b-styrene-bethylene oxide) Triblock Copolymers. Macromolecules 2002, 35, 7007−7017. (34) Salvatore, S. Optical Metamaterials by Block Copolymer SelfAssembly; Springer International Publishing, 2015. (35) Olmon, R. L.; Slovick, B.; Johnson, T. W.; Shelton, D.; Oh, S.H.; Boreman, G. D.; Raschke, M. B. Optical dielectric function of gold. Phys. Rev. B: Condens. Matter Mater. Phys. 2012, 86, 235147.

ACKNOWLEDGMENTS We thank Alexander Macfaden and Calum Williams for valuable comments on early versions of the manuscript. This research was supported through the Swiss National Science Foundation through the National Center of Competence in Research Bio-Inspired Materials and grant numbers 200021_163220 (to U.S.) and PZ00P2_168223 (to B.D.W.), the Adolphe Merkle Foundation, the Engineering and Physical Sciences Research Council (EPSRC) through the Cambridge NanoDTC EP/G037221/1, EP/L027151/1, and EP/ G060649/1, and ERC LINASS 320503 and from the European Union’s Horizon 2020 Research and Innovation Programme under the Marie Sklodowska-Curie grant agreement no. 706329 (to I.G.). Y.G. and U.W. thank the National Science Foundation (DMR-1409105) for ﬁnancial support.

■

REFERENCES

(1) Cai, W.; Shalaev, V. Optical Metamaterials; Springer, 2010. (2) Pendry, J. B. Negative refraction makes a perfect lens. Phys. Rev. Lett. 2000, 85, 3966−9. (3) Pendry, J. B.; Schurig, D.; Smith, D. R. Controlling Electromagnetic Fields. Science 2011, 1780, 1780−1782. (4) Poddubny, A.; Iorsh, I.; Belov, P.; Kivshar, Y. Hyperbolic metamaterials. Nat. Photonics 2013, 7, 948−957. (5) Boltasseva, A.; Shalaev, V. M. Fabrication of optical negativeindex metamaterials: Recent advances and outlook. Metamaterials 2008, 2, 1−17. (6) Soukoulis, C. M.; Wegener, M. Past achievements and future challenges in the development of three-dimensional photonic metamaterials. Nat. Photonics 2011, 5, 523−530. (7) Hur, K.; Francescato, Y.; Giannini, V.; Maier, S. A.; Hennig, R. G.; Wiesner, U. Three-dimensionally isotropic negative refractive index materials from block copolymer self-assembled chiral gyroid networks. Angew. Chem., Int. Ed. 2011, 50, 11985−11989. (8) Dolan, J. A.; Wilts, B. D.; Vignolini, S.; Baumberg, J. J.; Steiner, U.; Wilkinson, T. D. Optical Properties of Gyroid Structured Materials: From Photonic Crystals to Metamaterials. Adv. Opt. Mater. 2015, 3, 12−32. (9) Hsueh, H.-Y.; Yao, C.-T.; Ho, R.-M. Well-ordered nanohybrids and nanoporous materials from gyroid block copolymer templates. Chem. Soc. Rev. 2015, 44, 1974−2018. (10) Wu, L.; Zhang, W.; Zhang, D. Engineering Gyroid-Structured Functional Materials via Templates Discovered in Nature and in the Lab. Small 2015, 11, 5004−5022. (11) Vignolini, S.; Yufa, N. A.; Cunha, P. S.; Guldin, S.; Rushkin, I.; Stefik, M.; Hur, K.; Wiesner, U.; Baumberg, J. J.; Steiner, U. A 3D optical metamaterial made by self-assembly. Adv. Mater. 2012, 24, OP23−7. (12) Salvatore, S.; Demetriadou, A.; Vignolini, S.; Oh, S. S.; Wuestner, S.; Yufa, N. A.; Stefik, M.; Wiesner, U.; Baumberg, J. J.; Hess, O.; Steiner, U. Tunable 3D Extended Self-Assembled Gold Metamaterials with Enhanced Light Transmission. Adv. Mater. 2013, 25, 2713−2716. (13) Salvatore, S.; Vignolini, S.; Philpott, J.; Stefik, M.; Wiesner, U.; Baumberg, J. J.; Steiner, U. A high transmission wave-guide wire network made by self-assembly. Nanoscale 2014, 7, 2040−3372. (14) Demetriadou, A.; Hess, O. Analytic theory of optical nanoplasmonic metamaterials. Phys. Rev. B: Condens. Matter Mater. Phys. 2013, 87, 161101. (15) Oh, S. S.; Demetriadou, A.; Wuestner, S.; Hess, O. On the origin of chirality in nanoplasmonic gyroid metamaterials. Adv. Mater. 2013, 25, 612−7. (16) Bergman, D. J.; Stroud, D. Physical Properties of Macroscopically Inhomogenous Media. Solid State Phys. 1992, 46, 147−269. (17) Gaponenko, S. V. Introduction to Nanophotonics; Cambridge University Press: Cambridge, 2010. (18) Bánhegyi, G. Colloid Polym. Sci. 1986, 264, 1030−1050. 1896

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

Article pubs.acs.org/journal/apchd5

Gyroid Optical Metamaterials: Calculating the Eﬀective Permittivity of Multidomain Samples James A. Dolan,†,‡ Matthias Saba,§ Raphael Dehmel,‡,□ Ilja Gunkel,⊥ Yibei Gu,∥,# Ulrich Wiesner,∥ Ortwin Hess,§ Timothy D. Wilkinson,† Jeremy J. Baumberg,‡ Ullrich Steiner,⊥ and Bodo D. Wilts*,⊥ †

Department of Engineering, University of Cambridge, J.J. Thomson Avenue, Cambridge CB3 0FA, U.K. Nanophotonics Centre, Department of Physics, University of Cambridge, J.J. Thomson Avenue, Cambridge CB3 0HE, U.K. § Department of Physics, Imperial College, Prince Consort Road, London SW7 2BB, U.K. ⊥ Adolphe Merkle Institute, Chemin des Verdiers 4, 1700 Fribourg, Switzerland ∥ Department of Materials Science and Engineering, Cornell University, 330 Bard Hall, Ithaca, New York 14853-1501, United States ‡

S Supporting Information *

ABSTRACT: Gold gyroid optical metamaterials are known to possess a reduced plasma frequency and linear dichroism imparted by their intricate subwavelength single gyroid morphology. The anisotropic optical properties are, however, only evident when a large individual gyroid domain is investigated. Multidomain gyroid metamaterials, fabricated using a polyisoprene-b-polystyrene-b-poly(ethylene oxide) triblock terpolymer and consisting of multiple small gyroid domains with random orientation and handedness, instead exhibit isotropic optical properties. Comparing three eﬀective medium models, we here show that the specular reﬂectance spectra of such multidomain gyroid optical metamaterials can be accurately modeled over a broad range of incident angles by a Bruggeman eﬀective medium consisting of a random wire array. This model accurately reproduces previously published results tracking the variation in normal incidence reﬂectance spectra of gold gyroid optical metamaterials as a function of host refractive index and volume ﬁll fraction of gold. The eﬀective permittivity derived from this theory conﬁrms the change in sign of the real part of the permittivity in the visible spectral region (so, that gold gyroid metamaterials exhibit both dielectric and metallic behavior at optical wavelengths). That a Bruggeman eﬀective medium can accurately model the experimental reﬂectance spectra implies that small multidomain gold gyroid optical metamaterials behave both qualitatively and quantitatively as an amorphous composite of gold and air (i.e., nanoporous gold) and that coherent electromagnetic contributions arising from the subwavelength gyroid symmetry are not dominant. KEYWORDS: gyroid, optical metamaterial, eﬀective medium model, block copolymer, polymer self-assembly

E

permittivity and permeability in electromagnetic material design. Potential applications famously include cloaking devices and “superlenses”.2,3 However, of perhaps more immediate technological interest is the access to particularly large and small, or strongly anisotropic (e.g., hyperbolic), material parameters and their associated science and engineering.4 Whereas metamaterials that operate in the microwave regime have existed for decades, it is only relatively recently that

lectromagnetic metamaterials are artiﬁcially structured materials for which the electromagnetic response is a function of not only their chemical composition but also their structure.1 When the length scales of the constituent structural units are signiﬁcantly smaller than the wavelength of interest, the response of the metamaterial may be described by the homogenized eﬀective permittivity εeff(ω) and permeability μeff(ω). Metamaterials greatly expand the range of electromagnetic responses otherwise found in natural and synthetic bulk materials. They therefore oﬀer huge ﬂexibility to exploit exotic situations, or spatial arrangements of eﬀective © 2016 American Chemical Society

Received: June 14, 2016 Published: September 6, 2016 1888

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

Article

In this work, we investigate the optical properties of multidomain gold gyroid optical metamaterials fabricated from the alternating gyroid phase of a polyisoprene-bpolystyrene-b-poly(ethylene oxide) (ISO) triblock terpolymer. The specular reﬂection of the isotropic metamaterial is measured under a range of angles of incidence of light, and the resulting reﬂectance spectra are compared to those predicted by three of the simplest (and therefore most common) analytical eﬀective medium theories applicable to amorphous composites of spherical or ellipsoidal inclusions of one material in a host matrix of another. We show that a Bruggeman model with ellipsoidal inclusions is the only model considered that can reproduce the features present in the measured reﬂectance spectra of the investigated multidomain gold gyroid optical metamaterials and that such optical metamaterials behave substantially similarly to nanoporous gold.

advances in nanofabrication have allowed the manufacture of optical metamaterials.5 Due to the requirement that the structural units of a metamaterial be deeply subwavelength, ideally by an order of magnitude or more, optical metamaterials demand feature sizes on the length scale of tens of nanometers. However, many early top-down lithographic techniques either were intrinsically two-dimensional (e.g., a single material layer) or ventured into the third dimension only by tedious and nonscalable stacking of individual layers. These techniques are arguably still incapable of fabricating three-dimensional nanostructures over macroscopically large areas with suﬃcient speed and cost-eﬀectiveness to allow optical metamaterials to attain true technological relevance. Therefore, until recently, three-dimensional optical metamaterials presented a considerable challenge.6 Polymer self-assembly presents an alternative and particularly intriguing means by which to fabricate intricate one-, two-, and three-dimensional morphologies on the appropriate length scales, from which optical metamaterials may be replicated.7 Block copolymers are macromolecules consisting of two or more covalently linked homopolymers (“blocks”) that can microphase separate into various well-deﬁned morphologies due to the chemical dissimilarity between blocks. In block copolymers consisting of three distinct and sequential blocks (i.e., linear triblock terpolymers) one such morphology is the alternating gyroid: two single gyroid networks, each composed of one block, separated by a matrix of the third. The single gyroid is a continuous, chiral, and triply periodic cubic network with a constant mean curvature surface that is found in a range of natural and synthetic self-assembled systems.8 As the two single gyroid networks in the alternating gyroid are chemically distinct, it is possible to selectively remove just one such network and use the remaining voided terpolymer as a sacriﬁcial template for metal deposition.9,10 It was using this technique that Vignolini et al. fabricated the ﬁrst truly threedimensional self-assembled optical metamaterial: a gold single gyroid with a ∼50 nm unit cell size and 30% ﬁll fraction.11 Gyroid metamaterials possess a range of optical properties not exhibited by the pure metal, including an unambiguous optical anisotropy.8 Large individual domains exhibit a signiﬁcantly decreased plasma frequency and linear dichroism, evidenced by the shift of the extinction peak by up to 100 nm upon rotation under linearly polarized light.11 Both the plasma frequency and the linear dichroism are additionally a function of the unit cell size, ﬁll fraction, and dielectric environment.12,13 Although much is now known about the optical properties of gyroid metamaterials, suitable estimates of the eﬀective material parameters remain elusive, thereby hindering a true appraisal of the metamaterial’s potential utility. A trihelical metamaterial (THM) model of the gyroid as periodic disconnected helices allows the analytical derivation of the permittivity, permeability, and chiral coupling parameter.14,15 From these the plasma frequency of the metamaterial and its variation with unit cell size, ﬁll fraction, and dielectric environment can be successfully predicted.12 However, the THM model does not describe the linear dichroism of gyroid metamaterials, and the model is unsuitable to average over an ensemble of small domains of random orientation and handedness. It is therefore of great interest to correctly identify the eﬀective material parameters of gyroid metamaterials and to understand to what extent the ordered subwavelength structure continues to aﬀect the optical response when the macroscopic order is not long range.

■

EFFECTIVE MEDIUM THEORIES For a material that is homogeneous at a particular length scale, its physical properties may be described by a reduced set of eﬀective material parameters.16 Eﬀective medium theories are approximate analytical means to ascribe a homogeneous (although potentially anisotropic) material parameter, in this case εeff(ω), to a heterogeneous mixture of two or more components.1 Such theories are anticipated to hold when the inhomogeneity length scale of the material and the local variation in the electric ﬁeld are both signiﬁcantly smaller than the wavelength of interest.17 Although numerous approaches of varying complexity exist, the two considered in this work are arguably the most prevalent theories: the Maxwell−Garnett theory for spherical inclusions and the Bruggeman theory.1,17 Maxwell−Garnett Theory: Case of Spherical Inclusions. The simplest form of the Maxwell−Garnett eﬀective medium theory considers spherical inclusions of one material in a host matrix of another material (Figure 1a). The eﬀective permittivity is found by solving the following implicit equation:1 (ε1(ω) − ε2(ω))f1 ε2(ω) + (ε1(ω) − ε2(ω))A +

ε2(ω) − εeff (ω) =0 ε2(ω) + (εeff (ω) − ε2(ω))A

(1)

where εeff(ω) is the (isotropic) eﬀective permittivity of the composite, ε1(ω) is the permittivity of the ﬁrst component (the inclusion), ε2(ω) is the permittivity of the second component (the host), f1 is the volume fraction of the ﬁrst component, A is the depolarization factor (1/3 for spherical inclusions), and ω is frequency. The depolarization factor relates the dipole moment of a dielectric ellipsoid to the applied external electric ﬁeld and varies from 0 (disks) to 1 (wires). The above theory is strictly valid only when the volume ﬁll fraction of the inclusions is small. As a result, the above equation is not invariant under the transformation ε1 ↔ ε2 and f1 ↔ f 2. Asymmetric formulations such as this are only valid for low volume fractions of the polar phase (see, for example, Table 1 in ref 18). Nonetheless, the Maxwell−Garnett eﬀective medium theory should be considered due to its widespread usage and having previously been employed to justify the diﬀering behavior of gold gyroid metamaterials from an amorphous composite.11 1889

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

Article

composite, it is possible to extend the theory to take anisotropy of the inclusions into account. This is done by modeling such inclusions as aligned ellipsoids with semiaxes ak. In such a case the depolarization factor A in eq 2 is replaced by Ak =

a1a 2a3 2

∫0

∞

du (ak2

+ u)

(a12

+ u)(a 22 + u)(a32 + u)

where Ak is the depolarization factor for light linearly polarized along the kth axis of an aligned ellipsoidal inclusion. Note that the derived eﬀective permittivity is hence only valid for that same relative orientation of linearly polarized light and the eﬀective permittivity of the material is anisotropic (i.e., when all ellipsoidal inclusions are assumed to be aligned). However, it is also possible to deﬁne a macroscopically isotropic eﬀective permittivity while allowing for microscopic anisotropy if the ellipsoidal inclusions are assumed to be randomly oriented in the composite (Figure 1c). In such a case, the eﬀective permittivity is derived by solving the following implicit equation (see Supporting Information): 3

∑ k=1

=0

(3)

RESULTS An optical and electron micrograph of the multidomain gyroid metamaterial, the geometry of the experiment, and the resulting reﬂectance spectra for transverse magnetic (TM) and transverse electric (TE) polarizations of incident light are shown in Figure 2. The optical micrograph captured under linearly polarized light (Figure 2a) highlights the light orange color of the metamaterial, and the electron micrograph of an individual domain (Figure 2b) is consistent with the gyroid nanostructure previously observed for this terpolymer.11−13 The small size and multiplicity of the domains can be more clearly seen in Figure S1. Both TM (Figure 2d) and TE (Figure 2e) reﬂectance spectra are qualitatively similar to those of bulk gold (Figure S2), insofar as they exhibit low reﬂectance at shorter wavelengths and increased reﬂectance at longer wavelengths across all angles of incidence. (Note that in Figures 2−5, reﬂectance spectra are plotted on a log scale as they exhibit spectral features that span multiple orders of magnitude.) In bulk gold, these features are attributable to interband transitions and the plasma frequency, respectively. However, the measured spectra diﬀer quantitatively from those of bulk gold due to both a lowered eﬀective plasma frequency and their variation with angle of incidence. Otherwise, the spectra exhibit the general decrease (increase) in reﬂectance for

εeff (ω) + (ε1(ω) − εeff (ω))A =0

εeff (ω) + (ε2(ω) − εeff (ω))Ak

■

(ε1(ω) − εeff (ω))f1

εeff (ω) + (ε2(ω) − εeff (ω))A

(ε2(ω) − εeff (ω))f2

where εeff(ω), ε1(ω), ε2(ω), f1, f 2, and ω are as deﬁned above and Ak are the three depolarization factors corresponding to the geometry of the ellipsoidal inclusions (A1 + A2 + A3 = 1). Note that this equation is identical for both a polycrystalline sample consisting of numerous randomly oriented anisotropic domains and a composite sample consisting of equal amounts of three isotropic constituents of diﬀering permittivities or depolarization factors.16 Note also that the Maxwell−Garnett theory may similarly be extended to take into account microscopic anisotropy (vide inf ra).

Bruggeman Theory: Case of Spherical Inclusions. We adopt here a version of the Bruggeman eﬀective medium theory, in which all constituents of the composite are treated symmetrically. If the inclusions are again assumed to be spherical (Figure 1b), the eﬀective permittivity is found by solving the following implicit equation (see Supporting Information for more information):18

(ε2(ω) − εeff (ω))f2

εeff (ω) + (ε1(ω) − εeff (ω))Ak

+

Figure 1. Sketches of the mathematical representations of various eﬀective medium theories. (a) Maxwell−Garnett, eq 1, where the eﬀective permittivity (εeff) is derived by considering spherical inclusions (A = 1/3) of one material (ε1) in a host matrix of another (ε2). (b) Bruggeman (A = 1/3), eq 2, where the eﬀective permittivity (εeff) is derived by averaging over single inclusions (ε1 and ε2) individually embedded in an eﬀective medium consisting of all other inclusions (εeff). (c) Bruggeman (Ak), eq 3, where the eﬀective permittivity (εeff) is derived analogously to the case where A = 1/3 except that all individual spherical inclusions are replaced by randomly oriented ellipsoids. (d) The single gyroid morphology for which an eﬀective medium theory is sought.

+

(ε1(ω) − εeff (ω))f1

(2)

where εeff(ω), ε1(ω), ε2(ω), f1, A, and ω are deﬁned as above, and f 2 = 1 − f1 is the volume ﬁll fraction of the second component. Note that the above equation is now invariant under the transformation ε1 ↔ ε2 and f1 ↔ f 2, indicating that the Bruggeman eﬀective medium theory is applicable for any given volume ﬁll fraction. It is therefore anticipated that this simplest form of the Bruggeman theory may more accurately model the behavior of 30% ﬁll fraction gyroid metamaterials, such as those considered here. Bruggeman Theory: Case of Ellipsoidal Inclusions. Although the Bruggeman eﬀective medium theory is insensitive to the absolute size of the subwavelength inclusions of a 1890

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

Article

Figure 2. Gyroid optical metamaterials: optical and electron micrographs, experiment geometry, and measured reﬂectance spectra. (a) Optical micrograph of multidomain gold gyroid metamaterial under linearly polarized light (scale bar 100 μm). (b) Electron micrograph of an individual domain of the sample (scale bar 200 nm). (c) Specular reﬂectance spectra of the gyroid metamaterial are measured as a function of angle of incidence between 15° and 65° and 450 and 800 nm. Although a single gyroid domain is shown for clarity, the measurement spot size in fact encompasses a large number of randomly oriented gyroid domains. (d) Reﬂectance spectra as a function of angle of incidence for transverse magnetic (TM) polarized light (log color scale extends from −1.8 to −0.1). (e) The same for transverse electric (TE) polarized light (log color scale extends from −1.8 to −0.1).

Figure 3. Comparison of measured and modeled TM reﬂectance spectra as a function of angle of incidence using three eﬀective medium theories. (a) Measured reﬂectance spectra for transverse magnetic (TM) polarized light repeated from Figure 2d (log color scale extends from −1.8 to 0). (b) Reﬂectance spectra generated using the Maxwell−Garnett theory (log color scale extends from −6.0 to −1.0). (c) The same generated using the Bruggeman theory and A = 1/3, i.e., spherical inclusions (log color scale extends from −2.0 to −0.8). (d) The same generated using the Bruggeman theory and A1 = 0.66, A2 = 0.34, and A3 = 0, i.e., ellipsoidal inclusions (log color scales extends from −1.9 to −0.6).

TM (TE) polarized light with increasing angle of incidence, with an eﬀective Brewster’s angle of ∼50°. A comparison between the measured and modeled reﬂectance spectra across all wavelengths and angles of incidence for TM polarized light is shown in Figure 3; the same for TE polarized light is shown in Figure S3. The eﬀective permittivity εeff(ω) used to generate the modeled spectra in Figure 3b was calculated using the Maxwell−Garnett theory by setting ε1(ω) = εAu(ω), ε2(ω) = 1, f1 = 0.3, and A = 1/3 (i.e.,

spherical inclusions) in eq 1. Clearly the Maxwell−Garnett eﬀective medium theory is a poor model for the eﬀective permittivity of the gyroid metamaterial, as it predicts a striking dip in reﬂectance at an eﬀective Brewster’s angle of ∼60°, which is entirely absent in the measured data. Despite also assuming spherical inclusions, the eﬀective permittivity calculated using the Bruggeman theory, by again setting ε1(ω), ε2(ω), f1, and A as above in eq 2, results in a far better qualitative match between the measured and modeled 1891

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

Article

Figure 4. Variation in normal incidence reﬂectance spectra and plasma edge as a function of host refractive index. (a) Measured reﬂectance spectra at normal incidence for 30% ﬁll fraction gold gyroid metamaterials inﬁltrated with media of refractive indices 1.0 (solid line), 1.33 (dashed line), 1.5 (dotted-dashed line), and 1.7 (dotted line) and the associated plasma edge of each spectrum in nanometers (labeled vertical lines of the same style). Data are reproduced from Salvatore et al.12 (b) Modeled normal incidence reﬂectance spectra using the optimized Bruggeman model where ε2(ω) of eq 3 is set to 1.02 (solid line), 1.332 (dashed line), 1.52 (dotted-dashed line), and 1.72 (dotted line) and the associated plasma edge of each spectrum in nanometers (labeled vertical lines of the same style). (c) Plasma edge against refractive index of host for measured (Expt.) and modeled (Brugg.) spectra and the relationship predicted by the trihelical metamaterial (THM) model, reproduced from Salvatore et al.12

Figure 5. Variation in normal incidence reﬂectance spectra and plasma edge as a function of gold volume ﬁll fraction. (a) Measured normal incidence reﬂectance spectra of gold gyroid metamaterials with volume ﬁll fractions of 30% (solid line), 45% (dashed line), 60% (dotteddashed line), 75% (dotted line), and 90% (solid line with circles) and the associated plasma edge of each spectrum in nanometres (labeled vertical lines of the same style). Data reproduced from Salvatore et al.12 (b) Modeled normal incidence reﬂectance spectra using the optimized Bruggeman model where f1 of eq 3 is set to 0.30 (solid line), 0.45 (dashed line), 0.60 (dotted-dashed line), 0.75 (dotted line), and 0.90 (solid line with circles) and the associated plasma edge of each spectrum in nanometers (labeled vertical lines of the same style). (c) Plasma edge against volume ﬁll fraction of gold for measured (Expt.) and modeled (Brugg.) spectra and the relationship predicted by the trihelical metamaterial (THM) model, reproduced from Salvatore et al.12

reﬂectance spectra (Figure 3c). The global reﬂectance minimum at ∼50° between 450 and 500 nm is reproduced well. However, the spectra still exhibit a decrease in reﬂectance at long wavelengths and high angles of incidence, which is not present in the experimental data. This decrease in reﬂectance is absent in the reﬂectance spectra of Figure 3d, which uses our microscopically anisotropic Bruggeman theory. These spectra were modeled by setting ε1(ω), ε2(ω), and f1 as above and A1 = 0.66, A2 = 0.34, and A3 = 0 in eq 3. These depolarization factors were found by performing a constrained optimization to ﬁt the TM reﬂectance spectra generated by the model to the measured data (see Experimental Methods). A quantitative comparison of the goodness of ﬁt of each model is presented in Table 1. Cost functions f(A) (see Experimental Methods) are tabulated not only for TM but also for TE polarization using the depolarization factors derived from the TM measurements. Note that the cost function evaluated for TE polarization using the depolarization factors derived from the TM measurements (A1 = 0.66, A2 = 0.34, and A3 = 0) is only 0.66% larger than the same cost function evaluated for TE polarization using the depolarization factors derived from the TE measurements (A1 = 0.70, A2 = 0.30, and

Table 1. Table of Cost Functions f(A) (See Experimental Methods) Associated with the Various Eﬀective Medium Theories (model), Equations (eq), Polarizations (pol), and Vector of Depolarization Factors (A)a

a

model (eq)

pol

A

f(A)

Max.−Garn. (1) Brugg. (2) Brugg (3) Max−Garn (1) Brugg (2) Brugg (3)

TM

1/3 1/3 [0.66, 0.34, 0] 1/3 1/3 [0.66, 0.34, 0]

2.02 0.28 0.12 0.34 0.08 0.04

TE

A lower value of cost function indicates a better ﬁt.

A3 = 0). This would not in general be the case (e.g., for an anisotropic sample). Both ﬁts yield A3 = 0, which thus selects a wire (i.e., a uniaxially inﬁnitely extended ellipsoid) with an elliptical cross-section. It is therefore clear that the microscopically anisotropic Bruggeman model consisting of randomly oriented wire inclusions is the best of the three eﬀective medium models considered and that only a single set of 1892

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

■

depolarization factors, A1 = 0.66, A2 = 0.34, and A3 = 0, is appropriate to model both TM and TE measurements. A good model for the eﬀective permittivity of the gyroid metamaterial should be capable of reproducing not only the measured reﬂectance spectra presented in this work but also the previously reported behaviors as a function of refractive index of the host and volume ﬁll fraction of gold. Figure 4 compares measurements performed by Salvatore et al. on 30% ﬁll fraction gold gyroids inﬁltrated with various refractive index media with the optimized Bruggeman model.12 Following the convention in that work, each normal incidence spectrum is characterized by its plasma edge, the wavelength of the point of inﬂection of the reﬂectance spectrum. In the simplest Drude model of the permittivity of metals, the plasma wavelength is the wavelength at which the permittivity changes from positive to negative and is characteristic of the density and eﬀective mass of the free electrons in the particular metal. The plasma edge is not the plasma wavelength but behaves similarly and may be more readily and systematically identiﬁed from experimental data than the plasma wavelength (see for example Figure S6 of ref 12). Figure 4a reproduces the reﬂectance spectra measured by Salvatore et al. upon inﬁltration of the gyroid metamaterial with media of refractive indices nfill = 1.0, 1.33, 1.5, and 1.7 and indicates the plasma edge in each case (the labeled vertical lines). Note how the plasma edge is red-shifted with increasing host refractive index. Figure 4b plots equivalent normal incidence reﬂectance spectra derived using the optimized Bruggeman model with ε2(ω) of eq 3 set to n2fill, respectively. Again the plasma edge is red-shifted with increasing host permittivity. Although the measured and modeled plasma edges do not perfectly coincide, it is clear from Figure 4c that the modeled plasma edges are within experimental error for each refractive index. Therefore, despite the dissimilarity between the measured and modeled normal incidence reﬂectance spectra, the model successfully predicts the plasma edge of the gold gyroid metamaterial. Furthermore, the optimized Bruggeman model performs better in this respect than the trihelical metamaterial analytical model, also reproduced from Salvatore et al. and shown in Figure 4c.12 The results of the optimized Bruggeman model may also be compared to previously measured data where the volume ﬁll fraction of gold is varied. Figure 5a shows normal incidence reﬂectance spectra from Salvatore et al. as the volume ﬁll fraction of the gold gyroid is increased from 30% to 90%. Only four of the ﬁve plasma edges are shown, since those for the 75% and 90% ﬁll fraction gyroids are within 2 nm of one another. Whereas the plasma edge is red-shifted with increasing refractive index of the host, it is blue-shifted as the ﬁll fraction increases and the reﬂectance of the gyroid metamaterial tends toward that of bulk gold. Figure 5b plots equivalent normal incidence reﬂectance spectra calculated from the optimized Bruggeman model. Here only two of the ﬁve plasma edges are shown, as all of those corresponding to ﬁll fractions above 30% are extremely close (within 2 nm). Again the plasma edge is blue-shifted with increased ﬁll fraction, as it was in the measured spectra. However, as can be seen in Figure 5c, there is signiﬁcant deviation between the measured and predicted plasma edges for intermediate ﬁll fractions between about 40% and 70%. Outside of this region (i.e., at low and high ﬁll fractions) the optimized Bruggeman model performs well and is comparable with the THM model.

Article

DISCUSSION

The failure of the Maxwell−Garnett theory to describe multidomain gyroid samples is perhaps not surprising, since its validity is limited to a low volume fraction of spherical dielectric inclusions that are spatially separated. The gyroid samples considered here consist however of an interconnected, percolating network of gold struts. The better description of the experimental system by the Bruggeman model with spherical inclusions arises primarily from the fact that this model retains it validity for a high density of scatterers, expressed in the model by the ﬁll fraction. The results of Figure 3 indicate that a model based on an eﬀective medium approach is able to approximate the random multidomain gyroid network, despite the morphological dissimilarity. While a model with a larger number of free parameters (i.e., the three depolarization factors) is expected to improve the level of agreement with the data, it is revealing that ﬁts of both reﬂected TE and TM polarized light result always in zero values for one of the depolarization factors Ak. Since Ak < 1/3 corresponds to a prolate ellipse, with a divergence for Ak → 0, the optimization of the Bruggeman model with free Ak values results in an eﬀective medium consisting of randomly oriented wires of elliptical cross-section (see Figure 6 inset). While a random wire assembly is a better description than isolated individual scatterers for an interconnected gyroid network, the good agreement between ﬁt and data is nevertheless surprising given that the Bruggeman theory does not model well percolating networks.19 Although allowing for microscopic anisotropy within the Maxwell−Garnett model (i.e., ellipsoidal inclusions) might similarly improve upon the results of the equivalent model with spherical inclusions, this variant of the Maxwell−Garnett model would still suﬀer from a limited validity because of the high volume ﬁll fractions of our samples and was therefore not considered. Like the classical wire-grid metamaterial, the gold gyroid metamaterial is shown to exhibit a strongly red-shifted plasma edge.20 The eﬀective permittivity εeff(ω) derived from the Bruggeman theory with optimized depolarization factors, shown in Figure 6a, has a crossover of the real part of the permittivity just below 650 nm (arrow). In contrast, the real part of the permittivity of the constituent gold does not cross the zero axis at any wavelength in the visible (inset). Notwithstanding the eﬀect of losses associated with the imaginary part of the permittivity, the gold gyroid metamaterial therefore behaves as both a dielectric (λ ≲ 650 nm) and metal (λ ≳ 650 nm) in the visible. In the simple Drude model of the permittivity of a metal, this crossover is associated with the plasma frequency (plasma wavelength), an association that is hard to isolate in more complicated models (e.g., Drude− Lorentz) or experimentally measured permittivities. The previously introduced plasma edge is thus useful to characterize the optical response of the gyroid metamaterial, despite the lack of a direct correlation with prominent features in the permittivity plots. The variation of the predicted real part of the permittivity with refractive index of the host and ﬁll fraction of gold is shown in Figure 6b and c, respectively. Although quantitatively distinct, it is clear that the general behaviors of both the plasma edge (Figures 4c and 5c) and the crossover wavelength (Figure 6b and c) are broadly similar. On the basis of this and the good ﬁt of the Bruggeman model to the specular reﬂectance spectra, we conclude that gyroid metamaterials 1893

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

Article

and the volume ﬁll fraction of gold near the top surface, accounting for the diﬀerences in the reﬂectivity. The relative decrease in the long-wavelength reﬂectance at high angles of incidence predicted by the Bruggeman model, more prominent when spherical inclusions are assumed and not present in the data, may similarly be a result of the gyroid metamaterial having a somewhat larger volume ﬁll fraction of gold at its surface compared with that expected from a planar cut across the gyroid morphology. Incorrect ﬁll fractions during optimization of the depolarization factors may also help to explain the relative inaccuracy of the model at intermediate ﬁll fractions (i.e., between about 40% and 70%) compared to the relative accuracy of the same model with respect to increasing refractive index of the host. However, to note that the fabrication of gyroid metamaterials with increased ﬁll fraction and the accurate measurement of the ﬁll fraction are diﬃcult compared to inﬁltration of the metamaterial with varying refractive index media.12 Results of the former experiments should therefore be treated with some caution. Finally, whereas all of the eﬀective medium models considered are insensitive to the absolute size of the subwavelength inclusions, it is known that the optical properties of gold gyroid metamaterials vary with unit cell size.12 The results presented here are therefore limited to gold gyroids with a similar unit cell size (i.e., ∼60 nm), although the methodology can of course easily be extended to gold gyroids of other unit cell sizes. Despite the potential shortcomings of the relatively simple analytical models employed here, the application of more complicated analytical models would not alter the current conclusion: that multidomain gold gyroid optical metamaterials behave substantially as if they were nanoporous gold.

■

Figure 6. Eﬀective permittivity of small domain gyroid metamaterials derived from the Bruggeman eﬀective medium theory. (a) Real (solid line) and imaginary (dashed line) parts of the eﬀective permittivity εeff(ω) calculated using the Bruggeman theory by setting ε1(ω) = εAu(ω), ε2(ω) = 1, f1 = 0.3, A1 = 0.66, A2 = 0.34, and A3 = 0 in eq 3. The insets are a sketch of the equivalent structure corresponding to the optimized Bruggeman model and the real (solid line) and imaginary (dashed lines) part of the permittivity of bulk gold εAu(ω). (b) Variation of the real part of the eﬀective permittivity with refractive index of the host medium. (c) Variation of the same with volume ﬁll fraction of gold.

CONCLUSION

In this work, the eﬀective permittivity of multidomain gold gyroid metamaterials was estimated by comparing the results of three eﬀective medium theories to measured specular reﬂectance spectra over a range of angles of incidence. We show that a microscopically anisotropic Bruggeman theory with wire inclusions provides the best ﬁt to the data and that the optimized depolarization factors imply a composite of randomly oriented gold wires of elliptical cross-section. That the averaged optical properties of multidomain gyroid metamaterials are well described by an eﬀective medium theory, including their variation with refractive index of the host and volume ﬁll fraction of gold, contradicts previous assertions that the subwavelength structure necessarily alone distinguishes gold gyroid metamaterials from amorphous nanoporous gold.11 This result is surprising, given the experimental results obtained for large individual gyroid domains.11 In particular, the gyrotropic transmission along one of the chiral gyroid axes that was attributed to the self-inductance of plasmon-polariton modes is not captured by the eﬀective medium model. If symmetry-related eﬀects of the intricate gyroid structure do indeed contribute to the optical properties of a macroscopic sample consisting of numerous randomly oriented domains, it seems that this contribution is averaged out through the random alignment of the multidomain gyroid assembly, as also appears to be the case for gyroid photonic crystals.29,30

averaged over many randomly oriented domains behave similarly to amorphous composites of air and gold (i.e., dilute metals) and therefore possess a similar response to nanoporous gold fabricated, for example, by dealloying.21−28 Although the optimized Bruggeman model is successful in predicting the optical properties of multidomain gold gyroid optical metamaterials (allowing to conclude that their optical properties are similar to nanoporous gold), it is by no means perfect, and various dissimilarities exist between the measured and predicted spectra. Surprisingly, the measured reﬂectance spectra are generally higher than those predicted. This is most likely caused by the details of the gyroid surface. For example, surface reconstruction (i.e., local reorientation) of the terblock terpolymer during thermal annealing can alter the in-coupling of light into the gyroid network. Alternatively, the details of the gyroid fabrication process might aﬀect the surface roughness 1894

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

■

Article

A1 + A 2 + A3 = 1

EXPERIMENTAL METHODS Fabrication. Gold gyroid metamaterial fabrication has been detailed elsewhere.11−13,31 In brief, samples are prepared using substrates of ﬂuorine-doped tin oxide (FTO)-coated glass (Solaronix) that have been cleaned using a piranha etch and immersed for 15 s in a 0.2% solution (v/v) of octyltrichlorosilane (Sigma-Aldrich) in anhydrous cyclohexane (SigmaAldrich). An 80 kg/mol polyisoprene-b-polystyrene-b-poly(ethylene oxide) triblock terpolymer with block volume fractions of 30%, 53%, and 17%, respectively (synthesized by anionic polymerization as detailed elsewhere32,33), is spun from a 10% (w/w) anhydrous anisole (Sigma-Aldrich) solution at 1200 rpm, resulting in an approximately 1 μm thick ISO ﬁlm as measured by thin ﬁlm interferometry. Samples are subsequently thermally annealed under vacuum at 180 °C for 30 min (ramp rate 150 °C/h), then allowed to cool over approximately 12 h. The polyisoprene block is degraded by exposure to UV light (VWR International, 254 nm, ∼50 mW/cm2) for up to 2 h and removed by dissolution in ethanol. The resulting template is ﬁlled by electrodeposition of gold (Metalor ECF60 and 0.5% (v/v) E3 brightener) at a constant potential of −0.8 V following a nucleation step (a cyclic voltammetry scan at a rate of 0.05 V/s with vertex potentials of 0, −1.2, and 0 V). The three-electrode cell consisted of the FTO-coated glass substrate as the working electrode, an evaporated gold thin ﬁlm as the counter electrode, and a saturated calomel reference electrode. Gold is grown both within and atop the polymer template, and the layer of excess bulk gold is cleaved at the interface between the nanostructured and bulk gold using Kapton tape, to ensure a smooth top surface (i.e., low surface roughness). Following electrodeposition, the remaining polymer template was removed by exposure to oxygen plasma for approximately 10 min (Diener MRC 100 at 100% power). The resulting gold single gyroid has a unit cell size of ∼60 nm and a ﬁll fraction of 30%.11,12 Characterization. Optical characterization is performed using an automated reﬂection goniometer with a ﬁxed illumination arm (QP600-2-SR-BX 600 μm core ﬁber and HPX-2000 Ocean Optics xenon light source). The sample and detection arm are arranged in the θ−2θ conﬁguration such that whenever the sample is tilted by an angle θ, the detection arm is tilted by an angle 2θ. The spectra are recorded by coupling the reﬂected light into an optical ﬁber (QP230-2-XSR 230 μm core) connected to a spectrometer (Ocean Optics QE6500) and are normalized at all angles of incidence with respect to the reﬂectance of a silver mirror. Linear polarizers are placed at the output of the illumination ﬁber and at the input of the detection ﬁber, ﬁxed to the illumination and detection arms, respectively. Spectra are recorded at angles of incidence between 15° and 65° in steps of 1°. The procedure is repeated for both TE and TM polarizations in parallel conﬁgurations (i.e., aligned polarizer and analyzer). Model. Where an eﬀective medium model requires ﬁtting, the MATLAB optimization toolbox is used to minimize the cost function: f (A) =

1 N×M

where A = [A1, A2, A3], Ak is the kth depolarization factor, λi is the ith wavelength, θinj is the jth angle of incidence, N is the total number of wavelengths, M is the total number of angles of incidence, and Rexp(λi, θinj ) and Rmodel(λi, θinj , A) are the experimental and modeled reﬂectance spectra, respectively. The modeled reﬂectance spectra are in turn calculated from the Fresnel equations for reﬂection from a semi-inﬁnite nonmagnetic homogeneous medium for TE: TE R model (λ i ,

θjin ,

A) =

nair cos(θjin) − neff (λi , A) cos(θjtr)

2

nair cos(θjin) + neff (λi , A) cos(θjtr)

and TM: TM R model (λ i ,

θjin ,

A) =

neff (λi , A) cos(θjin) − nair cos(θjtr)

2

neff (λi , A) cos(θjin) + nair cos(θjtr)

polarized light, where nair and neff(λi, A) are the refractive indices of air and the eﬀective medium respectively, and θtrj is the jth (complex) transmitted angle calculated by Snell’s law, i.e., nair sin(θjin) = neff (λi , A) sin(θjtr)

The assumption that the gold gyroid metamaterial appears semi-inﬁnite (and that the derived eﬀective permittivity is insensitive to ﬁlm thickness) is based upon the thickness of the ﬁlm (∼1 μm), the unit cell size (∼60 nm), and previous studies of ﬁlm thickness eﬀects in gold gyroid optical metamaterials,34 which indicate that the reﬂectance spectra do not change beyond a threshold sample thickness. The eﬀective medium models from which neff(λi, A) is derived require as an input the permittivity of bulk gold, εAu(ω), which is here taken as that measured by Olmon et al.35 Optimized depolarization factors are calculated for each polarization state of light.

■

ASSOCIATED CONTENT

S Supporting Information *

The Supporting Information is available free of charge on the ACS Publications website at DOI: 10.1021/acsphotonics.6b00400. Additional data related to this publication is available at the University of Cambridge data repository (http://dx.doi.org/10.17863/CAM.4376). Supplementary Figures S1−S3 and details on the derivation of the Bruggeman eﬀective medium theory (PDF)

■

AUTHOR INFORMATION

Corresponding Author

*E-mail: [email protected] Phone: +41 (0)26 300 89 69.

N

Present Addresses

∑×

□

Papierfabrik Louisenthal GmbH, 83701 Gmund a.T., Germany. # The Dow Chemical Company, 2301 N. Brazosport Boulevard, Freeport, Texas 77541, United States.

i=1

M

∑ (log10R exp(λi , θjin) − log10R model(λi , θjin , A))2 j=1

Notes

The authors declare no competing ﬁnancial interest.

such that 1895

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896

ACS Photonics

■

Article

(19) Kirkpatrick, S. Percolation and conduction. Rev. Mod. Phys. 1973, 45, 574. (20) Pendry, J. B.; Holden, A. J.; Stewart, W. J.; Youngs, I. Extremely low frequency plasmons in metallic mesostructures. Phys. Rev. Lett. 1996, 76, 4773−4776. (21) Yu, F.; Ahl, S.; Caminade, A.-M.; Majoral, J.-P.; Knoll, W.; Erlebacher, J. Simultaneous excitation of propagating and localized surface plasmon resonance in nanoporous gold membranes. Anal. Chem. 2006, 78, 7346−50. (22) Dixon, M. C.; Daniel, T. A.; Hieda, M.; Smilgies, D. M.; Chan, M. H. W.; Allara, D. L. Preparation, structure, and optical properties of nanoporous gold thin films. Langmuir 2007, 23, 2414−22. (23) Maaroof, A. I.; Gentle, A.; Smith, G. B.; Cortie, M. B. Bulk and surface plasmons in highly nanoporous gold films. J. Phys. D: Appl. Phys. 2007, 40, 5675−5682. (24) Biener, J.; Nyce, G. W.; Hodge, A. M.; Biener, M. M.; Hamza, A. V.; Maier, S. A. Nanoporous Plasmonic Metamaterials. Adv. Mater. 2008, 20, 1211−1217. (25) Sardana, N.; Birr, T.; Schlenker, S.; Reinhardt, C.; Schilling, J. Surface plasmons on ordered and bi-continuous spongy nanoporous gold. New J. Phys. 2014, 16.06305310.1088/1367-2630/16/6/063053 (26) Sardana, N.; Heyroth, F.; Schilling, J. Propagating surface plasmons on nanoporous gold. J. Opt. Soc. Am. B 2012, 29, 1778. (27) Lang, X.; Qian, L.; Guan, P.; Zi, J.; Chen, M. Localized surface plasmon resonance of nanoporous gold. Appl. Phys. Lett. 2011, 98, 2009−2012. (28) Maaroof, A. I.; Cortie, M. B.; Smith, G. B. Optical properties of mesoporous gold films. J. Opt. A: Pure Appl. Opt. 2005, 7, 1464−4258. (29) Michielsen, K.; De Raedt, H.; Stavenga, D. G. Reflectivity of the gyroid biophotonic crystals in the ventral wing scales of the Green Hairstreak butterfly, Callophrys rubi. J. R. Soc., Interface 2010, 7, 765− 771. (30) Saba, M.; Wilts, B. D.; Hielscher, J.; Schröder-Turk, G. E. Absence of Circular Polarisation in Reflections of Butterfly Wing Scales with Chiral Gyroid Structure. Mater. Today: Proc. 2014, 1, 193− 208. (31) Farah, P.; Demetriadou, A.; Salvatore, S.; Vignolini, S.; Stefik, M.; Wiesner, U.; Hess, O.; Steiner, U.; Valev, V. K.; Baumberg, J. J. Ultrafast Nonlinear Response of Gold Gyroid Three-Dimensional Metamaterials. Phys. Rev. Appl. 2014, 2, 044002. (32) Bailey, T. S.; Pham, H. D.; Bates, F. A. Morphological Behavior Bridging the Symmetric AB and ABC States in the Poly(styrene-bisoprene-b-ethylene oxide) Triblock Copolymer System. Macromolecules 2001, 34, 6994−7008. (33) Bailey, T. S.; Hardy, C. M.; Epps, T. H.; Bates, F. S. A Noncubic Triply Periodic Network Morphology in Poly(isoprene-b-styrene-bethylene oxide) Triblock Copolymers. Macromolecules 2002, 35, 7007−7017. (34) Salvatore, S. Optical Metamaterials by Block Copolymer SelfAssembly; Springer International Publishing, 2015. (35) Olmon, R. L.; Slovick, B.; Johnson, T. W.; Shelton, D.; Oh, S.H.; Boreman, G. D.; Raschke, M. B. Optical dielectric function of gold. Phys. Rev. B: Condens. Matter Mater. Phys. 2012, 86, 235147.

ACKNOWLEDGMENTS We thank Alexander Macfaden and Calum Williams for valuable comments on early versions of the manuscript. This research was supported through the Swiss National Science Foundation through the National Center of Competence in Research Bio-Inspired Materials and grant numbers 200021_163220 (to U.S.) and PZ00P2_168223 (to B.D.W.), the Adolphe Merkle Foundation, the Engineering and Physical Sciences Research Council (EPSRC) through the Cambridge NanoDTC EP/G037221/1, EP/L027151/1, and EP/ G060649/1, and ERC LINASS 320503 and from the European Union’s Horizon 2020 Research and Innovation Programme under the Marie Sklodowska-Curie grant agreement no. 706329 (to I.G.). Y.G. and U.W. thank the National Science Foundation (DMR-1409105) for ﬁnancial support.

■

REFERENCES

(1) Cai, W.; Shalaev, V. Optical Metamaterials; Springer, 2010. (2) Pendry, J. B. Negative refraction makes a perfect lens. Phys. Rev. Lett. 2000, 85, 3966−9. (3) Pendry, J. B.; Schurig, D.; Smith, D. R. Controlling Electromagnetic Fields. Science 2011, 1780, 1780−1782. (4) Poddubny, A.; Iorsh, I.; Belov, P.; Kivshar, Y. Hyperbolic metamaterials. Nat. Photonics 2013, 7, 948−957. (5) Boltasseva, A.; Shalaev, V. M. Fabrication of optical negativeindex metamaterials: Recent advances and outlook. Metamaterials 2008, 2, 1−17. (6) Soukoulis, C. M.; Wegener, M. Past achievements and future challenges in the development of three-dimensional photonic metamaterials. Nat. Photonics 2011, 5, 523−530. (7) Hur, K.; Francescato, Y.; Giannini, V.; Maier, S. A.; Hennig, R. G.; Wiesner, U. Three-dimensionally isotropic negative refractive index materials from block copolymer self-assembled chiral gyroid networks. Angew. Chem., Int. Ed. 2011, 50, 11985−11989. (8) Dolan, J. A.; Wilts, B. D.; Vignolini, S.; Baumberg, J. J.; Steiner, U.; Wilkinson, T. D. Optical Properties of Gyroid Structured Materials: From Photonic Crystals to Metamaterials. Adv. Opt. Mater. 2015, 3, 12−32. (9) Hsueh, H.-Y.; Yao, C.-T.; Ho, R.-M. Well-ordered nanohybrids and nanoporous materials from gyroid block copolymer templates. Chem. Soc. Rev. 2015, 44, 1974−2018. (10) Wu, L.; Zhang, W.; Zhang, D. Engineering Gyroid-Structured Functional Materials via Templates Discovered in Nature and in the Lab. Small 2015, 11, 5004−5022. (11) Vignolini, S.; Yufa, N. A.; Cunha, P. S.; Guldin, S.; Rushkin, I.; Stefik, M.; Hur, K.; Wiesner, U.; Baumberg, J. J.; Steiner, U. A 3D optical metamaterial made by self-assembly. Adv. Mater. 2012, 24, OP23−7. (12) Salvatore, S.; Demetriadou, A.; Vignolini, S.; Oh, S. S.; Wuestner, S.; Yufa, N. A.; Stefik, M.; Wiesner, U.; Baumberg, J. J.; Hess, O.; Steiner, U. Tunable 3D Extended Self-Assembled Gold Metamaterials with Enhanced Light Transmission. Adv. Mater. 2013, 25, 2713−2716. (13) Salvatore, S.; Vignolini, S.; Philpott, J.; Stefik, M.; Wiesner, U.; Baumberg, J. J.; Steiner, U. A high transmission wave-guide wire network made by self-assembly. Nanoscale 2014, 7, 2040−3372. (14) Demetriadou, A.; Hess, O. Analytic theory of optical nanoplasmonic metamaterials. Phys. Rev. B: Condens. Matter Mater. Phys. 2013, 87, 161101. (15) Oh, S. S.; Demetriadou, A.; Wuestner, S.; Hess, O. On the origin of chirality in nanoplasmonic gyroid metamaterials. Adv. Mater. 2013, 25, 612−7. (16) Bergman, D. J.; Stroud, D. Physical Properties of Macroscopically Inhomogenous Media. Solid State Phys. 1992, 46, 147−269. (17) Gaponenko, S. V. Introduction to Nanophotonics; Cambridge University Press: Cambridge, 2010. (18) Bánhegyi, G. Colloid Polym. Sci. 1986, 264, 1030−1050. 1896

DOI: 10.1021/acsphotonics.6b00400 ACS Photonics 2016, 3, 1888−1896